Upload
others
View
1
Download
0
Embed Size (px)
Improvements to the Binary Phase Field Crystal
Theory with Applications in the Kinetics of
Precipitation
Nathan Frederick Smith
Department of PhysicsMcGill University, Montreal
Canada
September 10, 2017
A thesis submitted to McGill University in partial fulfillment of therequirements of the degree of Masters of Science
c© Nathan Smith 2017
Dedication
This thesis is dedicated to my family and friends. You made this research and this time in
my life possible.
i
Acknowledgements
This thesis was made possible with a support of many different people and resources. First
and foremost is the support of my research supervisor Prof. Nikolas Provatas whose drive
and enthusiasm for his research is paralleled only by his support and guidance in his teaching.
He gave me a world of questions I’ll never tire of considering, something I can never thank
him enough for.
I would also like to thank Prof. David Ronis, for many great discussions especially in
the murky waters of non-equilibrium statistical mechanics. His course notes and references
proved invaluable in the writting of this thesis (the appendix on generialized Einstein re-
lations most especially). About 7 years prior to the writing of this thesis, he entertained
my question ”How do you know if you’ve chosen the correct reaction co-ordinate?” in his
Introduction to Physical Chemistry course. It seems in retrospect that I haven’t stopped
asking that question.
Thank you Camille Bowness for being so supportive throughout this entire degree, for
many discussions over morning espresso or on the walk to campus. Thanks as well for your
help in translating the abstract.
I swarm of great people helped in the editting of this thesis including Quentin Stoyel,
Motoki Nakamura, Paul Jreidini and, of course, Nikolas Provatas. Thank you all for your
time. I can’t thank you enough for you patience and advice.
A huge thank you to my family and friends for supporting me while I took these years
to take a magnifying glass to the world. I couldn’t have done it without you.
Finally, this research was made possible with resources from Compute Canada and Calcul
Quebec and with funding from the Canada Research Chairs Program.
ii
Abstract
Two improvements to the binary Structural Phase Field Crystal (XPFC) theory are pre-
sented. The first is a general phenomenology for modelling density-density correlation func-
tions and the second extends the free energy of mixing term in the binary XPFC model
beyond ideal mixing to a regular solution model. These improvements are applied to study
kinetics of precipitation from solution. We see a two-step nucleation pathway similar to
recent experimental work [1, 2] in which the solution first decomposes into solute-poor and
solute-rich regions followed by nucleation in the solute-rich regions. Additionally, we find
a phenomenon not previously described in literature in which the growth of precipitates is
accelerated in the presence of uncrystallized solute-rich regions.
iii
Abrégé
Nous présentons deux ameliorations au theorie ”Structural Phase Field Crystal” (XPFC)
binaire. Le premier decrit une phénoménologie pour une modèle des fonctions de corrélations
des densités, et le deuxième augmente la modèle XPFC binaire au delà de la modèle idéale en
ajutant une terme au énergie libre de Helmholtz. Ces améliorations sont appliqués aux études
kinétiques de la précipité d’une solution. Nous voyons un chemin de nucléation similaire aux
éxpériments réçentes [1, 2] dans lequel le solution se sépare en regions avec concentration de
soluté bas et élèvé suivi par nucléation dans les régions avec hautes concentrations de soluté.
De plus, nous decouvrons une acceleration de l’acroissement du precipité en presence des
regions avec une concentration de soluté élèvé. Ce dernier est une phénomène auparavant
pas décrit en literature.
iv
Contents
Dedication i
Acknowledgements ii
Abstract iii
Abrégé iv
List of Tables x
1 Introduction 1
2 Introduction to Classical Density Functional Theory 5
2.1 Statistical Mechanics in the Semi-classical limit . . . . . . . . . . . . . . . . 6
2.1.1 Indistinguishability . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8
2.2 Classical Density Functional Theory . . . . . . . . . . . . . . . . . . . . . . . 10
2.3 Techniques in Density Functional Theory . . . . . . . . . . . . . . . . . . . . 14
3 Classical Density Functional Theory of Freezing 18
3.1 Amplitude Expansions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 19
3.2 Dynamic Density Functional Theory . . . . . . . . . . . . . . . . . . . . . . 23
3.2.1 Overview of Non-equilibrium Statistical Mechanics . . . . . . . . . . 23
3.2.2 Equation of Motion for the Density . . . . . . . . . . . . . . . . . . . 24
v
3.3 Phase Field Crystal Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . 27
4 Simplified Binary Phase Field Crystal Models 29
4.1 Binary PFC Background . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 29
4.2 Original Binary Phase Field Crystal Model . . . . . . . . . . . . . . . . . . . 31
4.3 Original Binary Structural Phase Field Crystal Model . . . . . . . . . . . . . 33
4.3.1 XPFC Correlation Functions . . . . . . . . . . . . . . . . . . . . . . . 35
5 Improvements to the Binary XPFC Model 38
5.1 Adding an Enthalpy of Mixing . . . . . . . . . . . . . . . . . . . . . . . . . . 38
5.2 Generalizing the Two-Point Correlation Function . . . . . . . . . . . . . . . 39
5.3 Equilibrium Properties of Binary Alloys . . . . . . . . . . . . . . . . . . . . 41
5.3.1 Eutectic Phase Diagram . . . . . . . . . . . . . . . . . . . . . . . . . 41
5.3.2 Syntectic Phase Diagram . . . . . . . . . . . . . . . . . . . . . . . . . 43
5.3.3 Monotectic Phase Diagram . . . . . . . . . . . . . . . . . . . . . . . . 44
6 Applications 46
6.0.1 XPFC Dynamics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 47
6.1 Multi-Step Nucleation of Nanoparticles in Solution . . . . . . . . . . . . . . 47
6.1.1 Classical and Non-classical Nucleation Theories . . . . . . . . . . . . 48
6.1.2 XPFC Modelling of Precipitation . . . . . . . . . . . . . . . . . . . . 49
6.1.3 Dynamics of Precipitation: Results and Discussion . . . . . . . . . . 51
6.2 Outlook and Future Applications . . . . . . . . . . . . . . . . . . . . . . . . 55
7 Conclusion 57
A Noise in Nonlinear Langevin Equations 59
A.1 Generalized Einstein Relations in an Arbitrary Model . . . . . . . . . . . . . 60
A.2 Example 1 - Model A . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 62
A.2.1 The partition function route . . . . . . . . . . . . . . . . . . . . . . . 63
vi
A.2.2 The Equation of Motion Route . . . . . . . . . . . . . . . . . . . . . 64
A.3 Example 2 - Time Dependent Density Functional Theory . . . . . . . . . . . 65
A.3.1 Pair Correlation from the Partition Functional . . . . . . . . . . . . . 65
A.3.2 Linearing the equation of motion . . . . . . . . . . . . . . . . . . . . 66
B Gaussian Functional Integrals 67
C Binary Correlation Functions 69
D Algorithms 72
D.1 Semi-Implicit Spectral Methods for Systems of First Order PDEs . . . . . . 72
D.2 Applications to the Binary XPFC Model . . . . . . . . . . . . . . . . . . . . 75
D.2.1 Algorithm for the Concentration c(x, t) . . . . . . . . . . . . . . . . . 76
D.2.2 Algorithm for the Total Density n(x, t) . . . . . . . . . . . . . . . . . 77
vii
List of Figures
3.1 Grand Potential through the Solidification transition . . . . . . . . . . . . . 21
4.1 Eutectic Phase Diagram with Metastable Projections . . . . . . . . . . . . . 36
5.1 Eutectic Phase Diagram . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 42
5.2 Syntectic Phase Diagram . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 44
5.3 Monotectic Phase Diagram . . . . . . . . . . . . . . . . . . . . . . . . . . . . 45
6.1 Coexistance Phase Diagram with Metastable Spinodal . . . . . . . . . . . . . 50
6.2 Stages of precipitation of nanoparticles from solution . . . . . . . . . . . . . 52
6.3 Droplet growth 〈R(t)〉 Versus time. Black line show ∼ t1/2 growth. Insets
show early hyper-diffusive growth of crystalline nanoparticles and late stage
hypo-diffusive growth. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 54
6.4 Fraction of uncrystallized droplets in time . . . . . . . . . . . . . . . . . . . 55
D.1 Schematic of time step . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 73
viii
List of Tables
3.1 Table of Ramakrishnan results . . . . . . . . . . . . . . . . . . . . . . . . . . 22
ix
List of Symbols
∗ Denotes an inner product (where appropriate) and integration over repeated variables.
b Bold font denotes a vector quantity.
β The inverse temperature 1/kbT where kb is Boltzmann’s constant.
ρ The average number density N/V . When refered to as a function ρ(x) it is the local
number density.
x
Chapter 1
Introduction
The study of alloys in materials physics is a pursuit of incredibly broad impact since the
functional properties of materials depend on their microstructure, which forms through non-
equilibrium phase transformations during the process of forming a material. As a result,
industries as diverse as those dealing in commercial products based on steel and aluminium
to the burgeoning markets dealing in nano-fabrication and optoelectronics are affected by
research in alloy materials. One of the most useful paradigms for understanding complex
alloy microstructure is that of the binary alloy.
One surprising aspect of binary alloys is the rich diversity of properties and behaviours
they display. Because material properties depend on the microstructural details of the ma-
terial, they have a strong processing path dependence. Grain boundaries, vacancies, disloca-
tions and other microstructural artifacts are all intimately tied to the manufacturing process
of the alloy. This means that the study of solids can never be completely separated from the
study of solidification. As such, the diversity of material properties and behaviours we see in
binary alloys can be directly attributed to the diversity of processes for their construction.
Given the importance of binary systems, it is critical to construct models that can explain
the diversity of behaviour we see in them. At the moment, models of alloy solidification can
be categorized by the length and time scales they accurately describe. At macroscopic length
1
and time scales, we have continuum methods of heat and mass transport and associated finite
element methods of analysis. These methods are appropriate for studying large castings, for
example. On length scales O(10−6m) to O(10−3m) we use Phase Field methods to study
phenomena such as dendritic growth and chemical segregation. On still finer length scales
fromO(10−9m) toO(10−6m) and on relatively long timescales, we have the methods of Phase
Field Crystal (PFC) theory and dislocation dynamics. These methods are appropriate for
studying nanoscopic changes that occur on diffusive timescales such as dislocation motion,
creep, grain boundary motion and micro segregation. At a still finer scale and on very short
time scales (O(10−12s)) we have the methods of molecular dynamics and density functional
theory. These methods are appropriate for the study of transport coefficients and interaction
potentials.
In this thesis, we’ll focus on extending a branch of binary PFC theory known as the
binary XPFC model –where the ”X” in XPFC signifies a class of PFC models constructed
to controllably simulate a robust range of metallic and non-metallic crystal symmetries com-
pared to the original PFC models. PFC binary models have been successful in describing a
broad selection of phenomena in binary alloys. These successes include eutectic and dendritic
solidification [3], the Kirkendall effect [4, 5], solute drag [6], clustering and precipitation [7–
9], colloidal ordering in drying suspensions [10], epitaxial growth and island formation [11,
12], and ordered crystals [13] to name a few.
The PFC theory is derived from Classical Density Functional Theory (CDFT) and as
such, it can be considered a simplified density functional theory. In practice, two different
variants of the PFC theory are used, as alluded to above: the original model developed
by Elder et al [3] and the Structural Phase Field Crystal (XPFC) model developed by
Greenwood et al. [14].
The original model was the first PFC theory of binary alloys and contains some impor-
tant physical properties of binary alloys. However, it is a very reduced form of CDFT and it
therefore lacks completeness in its ability to describe binary alloys. Specifically, the original
2
model uses an expansion in concentration that is actually a density difference not a concen-
tration, and the model has a limited ability to describe a realistic or robust range of phase
diagrams. The original model also uses a very simplified correlation kernel which limits its
ability to describe a variety of crystal lattice structures.
The XPFC model is an improvement that ameliorates the above problems. The con-
centration is left unexpanded allowing for construction of realistic global phase diagrams
instead of local expansions. More significantly, the XPFC model provides a phenomenology
for modelling two-point correlation functions that succeeded in describing solidification of
a variety of lattice structures, as well as transformations between different crystal lattices.
Simplifications of the multi-modal approach first introduced with the XPFC formalism has
been used to produce hexagonal, square, kagome, honeycomb, rectangular and other lattices
in 2 dimensions [15].
In introducing its phenomenology for modelling correlation functions, the binary XFPC
theory tacitly assumes that there is some preferred structure at high concentration and some
other structure preferred at low concentration. This assumption can be limiting in situations
that have a specific crystalline structure at intermediate concentrations, such as materials
with a syntectic phase diagram. At the syntectic point a solid of intermediate concentration
solidifies along the interface between a solute rich and solute poor liquid. The XPFC model
also assumes no long wavelength correlations in the concentration field which, in practice,
means the model has an ideal free energy of mixing. This is another limitation of the XPFC
model because the enthalpy of mixing is not generally zero for alloy systems.
The current research as three goals. The first goal is to improve the binary XPFC theory
by using a more general phenomenology for modelling pair correlation functions. The second
goal is another improvement to the binary XPFC theory which extends the free energy of
mixing beyond ideality to account for circumstances when the enthaply of mixing is not
negligible. The third goal is to use the new XPFC model derived herein to the elucidate the
multi-step nucleation process seen in certain diffusion-limited systems including gold and
3
silver nanoparticles [1].
The remainder of this thesis is divided into 5 chapters:
Chapter 2 Classical Density Functional Theory (CDFT) is introduced and derived from
fundamental principles of quantum statistical mechanics.
Chapter 3 CDFT theory of solidification is described and discussed. The density functional
theory is extended to a dynamic, non-equilibrium theory, and the Phase Field Crystal
(PFC) Theory is introduced from it as a simplified density functional theory.
Chapter 4 Binary PFC theory is derived and previous simplified alloy PFC models are
summarized and discussed.
Chapter 5 Improvements to the XPFC binary alloy theory are derived. This chapter con-
tains novel contributions to the field.
Chapter 6 The new XPFC alloy model derived herein is applied to model to the problem
of multi-step nucleation of nanoparticles from solution in diffusion limited systems and
potential future applications of this model are discussed.
4
Chapter 2
Introduction to Classical Density
Functional Theory
Many physical theories are derived using a succession of approximations. While each ap-
proximation yields a theory that is more narrow in scope, it is typically more tractable
to either analytical or numerical analysis. Classical Density Functional Theory (CDFT) is
derived using this approach and in this chapter we’ll examine each approximation and the
intermediate theory they supply.
CDFT is a theory of statistical mechanics. This means CDFT connects microscopic
physics to macroscopic observables using statistical inference1 instead of attempting to com-
pute microscopic equations of motion. The microscopic physics in this case is most accurately
described by many-body quantum mechanics and so the theory of quantum statistical me-
chanics is a natural starting point in any attempt to calculate thermodynamic observables.
We will see that for our systems of interest that the full quantum statistical theory is
completely intractable. To preceed, we’ll look at quantum statistical mechanics in the semi-
classical limit. In the semi-classical limit we’ll develop a theory of inhomogenous fluids called
Classical Density Functional Theory (CDFT). Finally, we’ll see that constructing exact free
1Statistical mechanics is not always described as statistical inference. See works of E. T. Jaynes for detailson this approach [16]
5
energy functionals for CDFT is rarely possible and look at an approximation scheme for
these functionals.
2.1 Statistical Mechanics in the Semi-classical limit
At a microscopic level, all systems are governed by the fundamental physics of quantum
mechanics. Statistical mechanics and in particular quantum statistical mechanics provides a
map between this microscopic reality and macroscopic thermodynamic observables. For most
applications, quantum statistical mechanics is both intractable to analysis and contains more
detail than necessary. For instance, the precise bosonic or fermionic nature of the particles
in the system often has little consequence on the thermodynamic properties. We can ignore
some of these quantum mechanical details by looking at statistical mechanics in the semi-
classical limit.
For the sake of clarity, we’ll look at a system of N identical particles in the canonical
ensemble which is straightforward to generalize to multi-component systems and other en-
sembles. We start with the definition of the partition function for a system of many particles,
Z = Tr[e−βĤ
], (2.1)
where,
Ĥ is the Hamiltonian |p̂|2
2m+ V (q̂),
p is set of particle momenta (p1, p2, ...pN),
q is similarly the set of particles positions, and,
β is the inverse temperature 1/kbT where kb is the Boltzmann constant.
Wigner [17], and shortly after, Kirkwood [18] showed that the partition function could be
expanded in powers of h̄, facilitating the calculation of both a classical limit and quan-
6
tum corrections to the partition function. Their method, the Wigner-Kirkwood expansion,
involves evaluating the trace operation over a basis of plane wave solutions,
Z(β) =∫
dqdp
(2πh̄)Ne−
ip·qh̄ e−βĤe
ip·qh̄ =
∫dΓI(q,p), (2.2)
Where, dΓ is the phase space measure dpdq/(2πh̄)N . To compute the integrand, I(q,p),
we follow Uhlenbeck and Bethe [19] and first compute its derivative,
∂I(q,p)
∂β= −e
ip·qh̄ Ĥe−
ip·qh̄ I(q,p). (2.3)
We then make a change of variables, I(q,p) = e−βHW (q,p), where H is the classical Hamil-
tonian. The new function W (q,p) encodes the deviation from classical behaviour due to a
lack of commutation of the potential and kinetic energy terms in the Hamiltonian. Substi-
tuting this redefined form of I(q,p) into equation 2.3, using the explicit form of the quantum
Hamiltonian and after a considerable amount of algebra we find a partial differential equation
for W ,
∂W
∂β=h̄2
2
(∇2q − β(∇2qV ) + β2(∇V )2 − 2β(∇qV ) · ∇q + 2
i
h̄p · (∇q − β∇q)
)W (q,p).
(2.4)
As in typical in perturbation theories, the solution can be expanded in a power series of a
small number, in this case, h̄, according to W = 1 + h̄W1 + h̄2W2 + .... By substituting this
expansion into I(q,p) = e−βHW (q,p) and I(p,q) back into equation 2.2 we find a power
series expansion for the partition function as well,
Z =(1 + h̄ 〈W1〉+ h̄2 〈W2〉+ ...
) ∫dΓeβH. (2.5)
7
Where the average, 〈·〉, denotes the the classical average,
〈A(p, q)〉 = 1Z
∫dΓA(p, q)e−βH. (2.6)
Solving equation 2.4 to second order in h̄ and computing the classical averages in equation
2.5 the quantum corrections to the classical partition are computed to second order as2,
〈W1〉 = 0, (2.7)
〈W2〉 = −β3
24m
〈|∇qV |2
〉. (2.8)
The first order term is zero because W1(q,p) is an odd function of p. In terms of the
Helmholtz free energy, for example, the corrections to second order would be,
F = Fclassical +h̄2β2
24m
〈|∇qV (q)|2
〉. (2.9)
There are a few items of importance in equation 2.9. First of all, the correction is
inversely proportional to both the temperature and the particle mass. For copper at room
temperature, for instance, the prefactor h̄2β2/(24m) is O(10−4) or at its melting temperature
the prefactor is O(10−6). The correction is also proportional to the mean of the squared force
felt by each particle. So high density materials will have a higher quantum correction because
they sample the short-range repulsive region of the pair potential more than their low density
counter parts.
2.1.1 Indistinguishability
There is an important distinction to be made between the quantum theory and the theory
in the semi-classical limit. The integral over phase space of the partition function must
only take into account the physically different states of the system. In the quantum theory
2For detailed calculations see [20].
8
this is achieved by tracing over any orthonormal basis of the Hilbert space, but in the
classical theory we need to be careful not to double count states involving identical particle
configurations. Classically, exchange of two identical particles does not result in a physically
different state and thus these states should be considered only once in the sum over states
in the partition function. More precisely, we should write the classical partition function as,
Z =∫ ′
dΓe−βH, (2.10)
Where the primed integral denotes integration only over the physically distinct states. In
the common case of N identical particles, the phase space integral becomes,
∫ ′dΓ→ 1
N !
∫dΓ (2.11)
Aggregating our results, we can thus write the partition function in the semi-classical limit
as,
Z(β) = 1N !
∫dΓe−βH +O(h̄2), (2.12)
Or, in the grand canonical ensemble,
Ξ(µ, β) =∞∑N=0
eβµN
N !
∫dΓ(e−βH +O(h̄2)
)(2.13)
Of course, to first order in h̄, this is exactly the form taught in introductory courses on
statistical mechanics and derived by Gibbs3 prior to any knowledge of quantum mechanics
[21]. The key insight here is to understand, in a controlled way, when this approximation is
accurate and the magnitude of the next quantum correction is as seen in equation 2.9. We
now apply this semi-classical limit of statistical mechanics to the study of the local density
field.
3The h̄ in Gibbs’ formula was justified on dimensional grounds and was simply introduced as a scalingfactor with units of action (J · s)
9
2.2 Classical Density Functional Theory
Ostensibly, when we study formation and evolution of microstructure in solids, our observable
of interest is the density field. As per usual in theories of statistical thermodynamics we must
distinguish between microscopic operators and macroscopic observables (the later being the
ensemble average of the former). In classical statistical mechanics, operators are simply
functions over the phase space, Γ. We use the term operator to make connection with the
quantum mechanical theory. In the case of the density field, the microscopic operator is the
sum of Dirac delta functions at the position of each particle,
ρ̂(x; q) =N∑i=0
δ(3) (x− qi) (2.14)
From which the thermodynamic observable is,
ρ(x) = 〈ρ̂(x; q)〉 = Tr [ρ̂(x; q)f(q,p)] (2.15)
Where, Tr [·] now denotes the classical trace,
Tr [A(q,p)f(q,p)] ≡∞∑N=0
1
N !
∫dΓA(q,p)f(q,p), (2.16)
And, f(q,p) is the equilibrium probability density function,
f(q,p) =e−β(H−µN)
Ξ(µ, β). (2.17)
where H is the classical Hamiltonian, µ the chemical potential of the system and Ξ(µ, β) is
the grand partition function of the system.
To construct a theory of the density field we review the usual methodology for statistical
thermodynamics. We will do so in the frame of entropy maximization in which the entropy
is maximized subject to the macroscopically available information. Taking the existence of
10
an average of the density field, particle number and energy as the macroscopically available
information, we can maximize then Gibb’s entropy functional,
S[f(q,p)] = −kbTr [f(q,p) ln (f(q,p))] , (2.18)
subject to the aforementioned constraints (fixed average density, particle number and total
energy) to find a probability density function of the form,
f(q,p) ∝ exp{−β(H− µN +
∫dxφ(x)ρ̂(x)
)}. (2.19)
Where, β, µ and φ(x) are the Lagrange multipliers associated with constraints of average
energy, number of particles and density respectively. As you might imagine, the constraints
of average particle number and density are not independent and satisfy,
N =
∫dxρ̂(x), (2.20)
We can combine their Lagrange multipliers into one,
f(q,p) ∝ exp(−β(H−
∫dxψ(x)ρ̂(x))
), (2.21)
Where, ψ(x) = µ− φ(x), is the combined Lagrange multiplier named the intrinsic chemical
potential. Recalling that chemical potential is the change in Helmholtz free energy made by
virtue of adding particles to the system,
∂F
∂N= µ, (2.22)
the interpretation of the intrinsic chemical potential follows as the Helmholtz free energy
change due to particles being added to a specific location. We’ll see this in more detail
briefly where we’ll see an analogous equation for the intrinsic chemical potential.
11
The objective of statistical theories is to compute the statistics of some observable (ran-
dom variable) of choice. Two special sets of statistics provide a complete description of
the observable’s probability distribution: the moments and cumulants4. The calculation of
moments and cumulants can be aided by use of generating functions. In the case of statis-
tical mechanics the generating functions of moments and cumulants have special physical
significance. The generating function of moments is closely related to the partition function
and the generating function of cumulants is closely related to the associated thermodynamic
potential.
In the case where the observable is the local density field, this is made somewhat more
technical by the fact that the density is a function instead of a scalar variable. As such
the partition function is more precisely called the partition functional as it depends on a
function as input. The thermodynamic potential will thus also be a functional. Specifically,
the grand canonical partition functional is,
Ξ[ψ(x)] = Tr
[exp
(−βH + β
∫dxψ(x)ρ̂(x)
)]. (2.23)
As alluded to above, the partition functional is a type of moment generating functional in
the sense that repeated (functional) differentiation with respect to the intrinsic chemical
potential yields moments of the density field:
β−n
Ξ
δnΞ[ψ]
δψ(x1) . . . δψ(xn)= 〈ρ̂(x1) . . . ρ̂(xn)〉 . (2.24)
Similarly, we can construct a thermodynamic potential by taking the logarithm of the parti-
tion function. This potential in particular is called the grand potential functional in analogy
with the grand potential of thermodynamics,
Ω[ψ(x)] = −kbT log (Ξ[ψ(r)]) . (2.25)4See [22] for discussion of moments, cumulants and their importance in statistical mechanics
12
The grand potential functional is a type of cumulant generating functional in the sense that
repeated functional differentiation yields cumulants of the density field:
−β−n+1 δnΩ[ψ]
δψ(x1) . . . δψ(xn)= 〈ρ̂(x1) . . . ρ̂(xn)〉c (2.26)
Where, 〈·〉c, denotes the cumulant average [22].
If we examine the first two cumulants,
− δΩ[ψ]δψ(x)
= 〈ρ̂(x)〉 ≡ ρ(x), (2.27)
−kbTδ2Ω[ψ]
δψ(x)δψ(x′)= 〈(ρ̂(x)− ρ(x))(ρ̂(x′)− ρ(x′))〉 , (2.28)
we notice two remarkable things: The first, implies that the average density field is a function
of only its conjugate field, the intrinsic chemical potential, and the second implies that that
relationship is invertible5. To see this, we compute the Jacobian by combining equation 2.27
and 2.28,
δρ(x)
δψ(x′)= β 〈(ρ̂(x)− ρ(x))(ρ̂(x′)− ρ(x′))〉 . (2.29)
The right hand side of equation 2.29 is an autocorrelation function and therefore positive
semi-definite by the Weiner-Khinchin theorem [23]. This implies that, at least locally, the
intrinsic chemical potential can always be written as a functional of the average density,
ψ[ρ(x)], and vice versa. Furthermore, because all of the higher order cumulants of the
density depend on the intrinsic chemical potential, they too depend only on the average
density.
Given the importance of the average density, ρ(x), it follows that we would like to use
a thermodynamic potential with a natural dependence on the density. We can construct a
generalization of the Helmholtz free energy that has precisely this characteristic by Legendre
5The inverse function theorem only implies local invertibility, there is no guarentee of global invertibility.Indeed phase coexistance is a manifestation of this fact where a single intrinsic chemical potential is sharedby two phases
13
transforming the Grand potential,
F [ρ(x)] = Ω[ψ[ρ]] +∫dxρ(x)ψ(x). (2.30)
F [ρ(x)] is called the intrinsic free energy functional.
It can be shown [24] that ρ(x) must be the global minimum of the grand potential, which
sets the stage for the methodology of classical density functional theory: if we have a defined
intrinsic free energy functional, F , we can find the equilibrium density field by solving the
asssociated Euler-Lagrange equation,
δΩ[ρ]
δρ(r)= 0. (2.31)
Finally, we may construct an analogous equation to equation 2.22 for the intrinsic chem-
ical potential,
δFδρ(x)
= ψ(x), (2.32)
which follows from equation 2.30 assuming equation 2.31. Equation 2.32 implies that the
intrinsic chemical potential is the free energy cost of adding density to the location x specif-
ically.
2.3 Techniques in Density Functional Theory
The difficulty in formulating a density functional theory is the construction of an appropriate
free energy functional. While exact calculations are rarely feasible, there are a variety of
techniques that help in building approximate functionals. It is important to note first what
we can compute exactly. In the case of the ideal gas, we can compute the grand potential
14
and free energy functional exactly,
Ωid[ψ] = −kbT
Λ3
∫dx eβψ(x) (2.33)
Fid[ρ] = kbT∫
dx{ρ(x) ln
(Λ3ρ(x)
)− ρ(x)
}, (2.34)
Where Λ is the thermal de Broglie wavelength,
Λ =
√2πh̄2
mkbT. (2.35)
We may then express deviation from ideality by factoring the ideal contribution out of the
partition function,
Ξ[ψ] = Ξid[ψ]Ξex[ψ], (2.36)
leading to grand potential and free energy functionals split into ideal and excess components,
Ω = Ωid + Ωex (2.37)
F = Fid + Fex. (2.38)
The interaction potential, V (q), in the excess partition function typically makes a direct
approach to calculating the excess free energy intractable. Though perturbative methods,
including the cluster expansion technique [25], have been developed to treat the interaction
potential systematically, other approximation schemes for the excess free energy are typically
more pragmatic, particularly where deriving models that are tractable for the numerical
simulation of dynamics is concerned. In particular, we can approximate the excess free
energy by expanding around a reference homogeneous fluid with chemical potential µ0 and
density ρ0,
Fex[ρ] = Fex[ρ0] +δFexδρ(x)
∣∣∣∣ρ0
∗∆ρ(x) + 12
∆ρ(x′) ∗ δ2Fex
δρ(x)δρ(x′)
∣∣∣∣ρ0
∗∆ρ(x) + . . . , (2.39)
15
where ∆ρ(x) = ρ(x) − ρ0 and we have introduced the notation, ∗ to mean integration over
repeated co-ordinates, for example,
f(x′) ∗ g(x′) ≡∫
dx′f(x′)g(x′). (2.40)
The excess free energy is the generating functional of a family of correlation functions called
direct correlation functions,
δnFex[ρ]δρ(x1)...δρ(xn)
= −βCn(x1, . . . , xn), (2.41)
the first of which, for a uniform fluid, is the excess contribution to the chemical potential.
We may express this as the total chemical potential less the ideal contribution (see equation
2.34),
δFexδρ
∣∣∣∣ρ0
= µex0 = µ0 − µid = µ0 − kbT ln(Λ3ρ0
). (2.42)
Truncating the expansion in equation 2.39 to second order in ∆ρ(x) and substituting the
linear and quadratic terms from equation 2.42 and 2.41, we can simplify the excess free
energy to,
Fex[ρ(r)] = Fex[ρ0]+∫dr{µ− kbT ln
(Λ3ρ0
)}∆ρ(r)−kbT
2∆ρ(r)∗C(2)0 (r, r′)∗∆ρ(r′), (2.43)
where C(2)0 (r, r
′) denotes the two-point direct correlation function at the reference state.
Combining equation 2.34 with the simplified excess free energy in equation 2.43, we can
express total change in free energy, ∆F = F − F [ρ0], as,
∆F [ρ(r)] = kbT∫
dr
{ρ(r) ln
(ρ(r)
ρ0
)− (1− βµ0)∆ρ(r)
}− kbT
2∆ρ(r) ∗C(2)0 (r, r′) ∗∆ρ(r′).
(2.44)
16
We find an equivalent expression for the grand potential after a Legendre transform,
∆Ω[ρ(r)] = kbT
∫dr
{ρ(r)
[ln
(ρ(r)
ρ0
)+ βφ(r)
]−∆ρ(r)
}− kbT
2∆ρ(r)∗C(2)0 (r, r′)∗∆ρ(r′),
(2.45)
where φ(r) is defined as an external potential, introduced into the system for completeness.
We see that the density functional theory derived here can be derived through a series
of approximations from a fundamental basis in quantum statistical mechanics and requires
no more parameters than the thermodynamic details of a homogeneous reference fluid. It
is reasonable to ask at this point whether or not we have really gained anything with this
approximation scheme. Although we have arrived at a relatively simple form for the free
energy functional, we’ve added several parameters to the functional based on the reference
fluid. Thankfully, the theory of homogeneous liquids is very well established. This implies
we may rely on a broad choice of analytical, numerical or experimental techniques to derive
these parameters.
Equation 2.44 establishes an approximate density functional theory for inhomogenous
fluids. However, as we will see in the following chapter, the properties of the direct correlation
function C2o (r, r′) also carries information about how the fluid solidifies in the solid state as
temperature or density cross into the coexistence.
17
Chapter 3
Classical Density Functional Theory
of Freezing
The classical density functional theories derived in chapter 2 were first established to study
inhomogenous fluids. By considering the solid state as an especially extreme case of an
inhomogeneous fluid [26], we can use CDFT to study the process of solidification. From the
perspective of CDFT, solidification occurs once the density field develops long range periodic
structure. While not expressed in precisely this language, this approach dates back as far as
1941 with the early work of Kirkwood and Monroe [27] and was later significantly refined
by Yussouff and Ramakrishnan [28].
We’ll see that the approach of Youssof and Ramakrishnan was very successful at ex-
plaining the solidification in the thermodynamic sense. That is to say, it elucidates the
parameters responsible for solidification but not the dynamical pathway responsible for the
transition. To discuss the pathway toward equilibrium and the non-equilibrium artifacts in-
troduced along the way into many solids (e.g. grain boundaries, vacancies, dislocations, etc)
we proceed to extend the CDFT framework using the Dynamic Density Functional Theory
(DDFT). Noting that the full DDFT framework can be intractable in practice, we conclude
by introducing a simplified density functional theory called the Phase Field Crystal (PFC)
18
theory.
3.1 Amplitude Expansions
To explore the problem of solidification, we begin with the approximate grand potential
established in equation 2.45 with the external potential, φ(r), set to zero,
β∆Ω[ρ(r)] =
∫dr
{ρ(r) ln
(ρ(r)
ρ0
)−∆ρ(r)
}− 1
2∆ρ(r) ∗ C(2)0 (r, r′) ∗∆ρ(r′). (3.1)
To make our theory concrete we must choose a suitable reference liquid to set the parameters
ρ0 and C(2)0 (r, r
′). We will choose the reference liquid to be the liquid at the melting point
with density ρl.
Scaling out a factor of ρl we can rewrite the grand potential in terms of a dimensionless
reduced density, n(r) ≡ (ρ(r)− ρl)/ρl,
β∆Ω[n(r)]
ρl=
∫dr {(1 + n(r)) ln (1 + n(r))− n(r)} − 1
2n(r) ∗ ρlC(2)0 (r, r′) ∗ n(r′). (3.2)
To approximate the density profile in the solid state we can expand the density in a plane
waves,
n(r) = n̄+∑G
ξGeiGr. (3.3)
Where {G} is the set of reciprocal lattice vectors in the crystal lattice and the amplitudes,
ξG, serve as order parameters for freezing. n̄ is the k = 0, or equivalently the spatial average,
of the density profile. In the liquid phase all amplitudes are zero and the average density is
uniform, while in the solid phase there are finite amplitudes that describe the periodic profile
of the crystal lattice. As we have chosen the reference fluid to be the liquid at the melting
point with uniform density ρl, n̄ is zero for the liquid phase at the melting point (for that
reference density) and n̄ is the fractional density change of solidification, defined here as η,
19
for the solid phase at the melting point, where
η =ρs − ρlρl
, (3.4)
and in which ρs is the macroscopic density of the solid phase.
The amplitudes are constrained by the point group symmetries of the lattice. Grouping
the amplitudes of symmetry-equivalent reciprocal lattice vectors together we can write the
density profile as,
n(r) = n̄+∑α
ξα ∑{G}α
eiG·x
, (3.5)Where α is a label running over sets of symmetry-equivalent reciprocal lattice vectors. More
precisely, if we apply the projection operator of the totally symmetric representation of
the lattice point group to the reciprocal lattice vectors we may label the distinct linear
combinations 1 with α [29]. The members of these distinct linear combinations form the set
{G}α.
If we insert equation 3.5 into equation 3.2 and integrate over the unit cell of the particular
crystal we wish to develop the theory for, we find,
β∆Ωcellρl
=
∫cell
dr {(n(r) + 1) ln (n(r) + 1)− n(r)}
− 12
[n̄2ρlC̃
(2)0 (0) +
∑α
ρlC̃(2)0 (Gα)λα|ξα|2
], (3.6)
Where λα is the number of reciprocal lattice vectors in the set α and C̃(2)0 (k) is the Fourier
transform of the direct correlation function of the reference fluid. The first term in equation
3.6 is convex in all of the amplitudes with a minimum at zero. It is noteworthy, as we will
discuss shortly, that the product ρlC̃(2)0 (Gα) is a simple function of the structure factor,
1These linear combinations are all formally equal to zero. It is important to treat opposite vectors (vand −v) as distinct for the sake of calculating the set {G}α.
20
S(k)2, namely,
ρlC̃20(k) =
S(k)− 1S(k)
∀ k 6= 0. (3.7)
It follows that solidification must occur when the product ρlC̃(2)0 (Gα) (or equivalently, the
reference structure factor S0(Gα)) is large enough to stabilize a finite amplitude by creating
a new minimum away from zero. This phenomenon is shown schematically in figure 3.1
where the grand potential is projected on to a particular ξα axis and plotted for different
values of the reference structure factor. When the reference structure factors are less than
some set of critical structure factors (denoted as S∗(Gα)), only zero amplitude solutions are
stable. When the reference structure factors are critical both the zero and non-zero amplitude
solutions are stable and we find liquid-solid coexistence. Once the reference structure factors
are greater than critical one the periodic crystalline solutions is stable.
Figure 3.1: Schematic view of the grand potential β∆Ω/ρl projected on to an ξα axis forthree different reference structure factors. To minimize the grand potential, finite ξα is stableonce S0(Gα) > S
∗(Gα)
Furthermore, equation 3.6 suggests that the set of critical structure factors, {S∗(Gα)}α
are material independent as no free parameters remain in the grand potential. As a con-
2This follows from the definition of the structure factor and the Ornstein-Zernike equation
21
sequence, once we specify the symmetry of the lattice a liquid will solidify into (eg. face-
centred-cubic), all materials that undergo this transition should share these parameters at
the melting point.
Early numerical evidence of this result was supplied by the Hansen-Verlet criterion [30]
which states that for a Lennard-Jones fluid the peak of the structure factor is constant along
the melting curve with a value ≈ 2.85. It has been noted that in comparing experimental
evidence of a variety of liquids solidifying to fcc structure, most have a peak value close to
2.8 whereas those solidifying into bcc structures have a peak value around 3.0 [28].
At this level, the CDFT theory of solidification is an infinite order parameter theory
of solidification. We can simplify the theory by truncating the number of amplitudes we
keep in our expansion of the density. This is justified by noting that only terms from the
first few reciprocal lattice families contain the majority of the grand potential energy of
solidification[28].
Theory C̃(G[111]) C̃(G[311]) ηI 0.95 0.0 0.074II 0.65 0.23 0.270III 0.65 0.23 0.166Experiment 0.65 0.23 0.148
(a) Freezing parameters for fcc withcomparison to Argon experimental re-sults.
Theory C̃(G[110]) C̃(G[211]) ηI 0.69 0.00 0.048II 0.63 0.07 0.052III 0.67 0.13 0.029Experiment 0.65 0.23 0.148
(b) Freezing parameters for bcc withcomparison to Sodium experimental re-sults.
Table 3.1: Freezing parameters for fcc and bcc systems and comparison to experiment from[28]. Theory I uses one order parameter, theory II uses two order parameters and theory IIIuses two order parameters with a higher (third) order expansion in the free energy. η is thefractional density change of solidification from equation 3.4
As seen in table 3.1a and table 3.1b theoretical results from a single amplitude theory
(theory I in the results) are poor but improve significantly with two order parameters (theory
II) or higher order expansions of the free energy (theory III).
22
3.2 Dynamic Density Functional Theory
In spite of its successes, the CDFT theory of solidification cannot be a general description of
solidification as many materials never fully reach equilibrium. The resulting microstructure
affects the mechanical properties of the solid. In order to improve our theory we need to
examine the pathway systems take to equilibrium so we can understand these microstructural
features. We begin with a brief overview of non-equilibrium statistical mechanics.
3.2.1 Overview of Non-equilibrium Statistical Mechanics
Consider a non-equilibrium probability distribution over phase space, f(q,p; t). As a func-
tion over phase space, its equation of motion is a simple result of classical mechanics,
df
dt= {f,H}+ ∂f
∂t. (3.8)
Where {·, ·} denotes the Poisson bracket,
{f, g} =N∑i=0
∂f
∂qi
∂g
∂pi− ∂g∂qi
∂f
∂pi. (3.9)
Of course, the distribution must remain normalized in time and therefore the total time
derivative must be zero, ∫dqdp f(q,p; t) = 1→ df
dt= 0. (3.10)
Accounting for this conservation law in equation 3.8, the resulting equation of motion is
called the Liouville Equation,
∂f
∂t= −{f,H} (3.11)
23
Under appropriate conditions the probability distribution, under the action of the Liouville
Equation, will decay to a stable fixed point feq(q,p) we call equilibrium,
limt→∞
f(q,p; t) = feq(q,p) (3.12)
Using the non-equilibrium probability distribution, we can also discuss non-equilibrium
averages of the density profile and their associated equations of motion. The non-equilibrium
density is written in analogy with equation 2.15 by taking of the classical trace of the density
operator over with the non-equilibrium distribution,
ρ(x, t) = 〈ρ̂(x; q)〉ne = Tr [ρ̂(x; q)f(q,p, t)] . (3.13)
Where 〈·〉ne denotes the non-equilibrium average, (i.e., using f(q,p, t)). Just as the non-
equilibrium probability distribution is driven to equilibrium by the Liouville Equation, so
too is the density profile by its own equation of motion.
3.2.2 Equation of Motion for the Density
A variety of equations of motion for the density field are known. For instance, we can consider
the Navier-Stokes equations of hydrodynamics as one such equation of motion. If we restrict
ourselves to diffusion limited circumstances, we may derive a much simpler equation of
motion. To achieve this result we use the projection operator method, and assume that the
density operator is the only relevant variable. Quoting the result from [23] we find,
∂ρ(r, t)
∂t= ∇ ·
[∫dr′D(r, r′, t) · ∇′ δF [ρ]
δρ(r′, t)
], (3.14)
where ∇′ denotes differentiation with r′, and D(r, r′, t) is the diffusion tensor,
D(r, r′, t) =
∫ ∞0
dτ ′Tr[f(q,p, t)Ĵ(r, 0)Ĵ(r′, τ ′)
], (3.15)
24
in which Ĵ(r, t) is the local density flux,
Ĵ(r, t) ≡N∑i
pimiδ(r − qi). (3.16)
Theories using equation 3.14 and variations thereof are often called Dynamic Density Func-
tional Theories (DDFT) or at times Time Dependent Density Functional Theories (TDDFT)
though we will use the former throughout this work.
The non-equilibrium diffusion tensor presents a significant impediment to integrating
this equation of motion so in practice it is often approximated. Following [23], if we assume
that the positions evolve more slowly than the velocities and that the momenta of different
particles are uncorrelated we can dramatically simplify the diffusion tensor,
D(r, r′) = D01ρ(r, t)δ(r − r′). (3.17)
Where D0 is the diffusion coefficient,
D0 =1
3m2
∫ ∞0
dtTr [f(q,p, t)pi(0) · pi(t)] . (3.18)
Substituting into equation 3.14 we find a simplified equation of motion originally suggested
by [31],
∂ρ(r, t)
∂t= ∇ ·
[D0ρ(r, t)∇
δF [ρ]δρ(r, t)
]. (3.19)
The equation of motion can also be written as a Langevin equation. In this variant
the equation of motion is for the density operator, ρ̂, and the noise is assumed to obey a
25
generalized Einstein relation,
∂ρ̂(x, t)
∂t= ∇ ·
[D0ρ̂(x, t)∇
(δF [ρ̂]δρ̂
)]+ ξ(x, t), (3.20)
〈ξ(x, t)〉 = 0, (3.21)
〈ξ(x, t)ξ(x′, t′)〉 = −2∇ · [D0ρ(x, t)∇δ(x− x′)δ(t− t′)] . (3.22)
See Appendix A for more details on generalized Einstein relations and [32] for a detailed
discussion about equations 3.19 and 3.20.
At times, the diffusion tensor is assumed to be constant. This is common place in many
Phase Field Crystal theories. In light of equation 3.19, this is akin to assuming the density
variations are small.
Unfortunately, if we were to use the approximate free energy functional established in
equation 2.44 in the DDFT of equation 3.19 or 3.20 we would face a major impediment:
the solid state solutions of the density functional theory approach yield sharply peaked
solutions at the position of the atoms in the lattice. While this is realistic, they are a major
challenge for numerical algorithms that aim to explore long-time microstructure evolution.
The challenges are two-fold. First, these sharp peaks require a fine mesh to be resolved
resulting in intractably large memory requirement to simulate domains of any non-trivial
scale. Second, linear stability analysis of most algorithms demonstrates that the time step
size is a monotonically increasing function of the grid spacing, thus only small time steps can
be taken on a fine mesh. This further restricts the time scales of microstructure evolution
that can be practicality explored to times scales comparable to those of molecular dynamics
–perhaps somewhat longer.
One pragmatic solution to this problem is to further approximate the free energy func-
tional of equation 2.44 in such a way as to produce a theory that retains the essential physics
of solidification but produces a solid state that is more smoothly peaked. As we will see next,
the Phase Field Crystal (PFC) theory, the topic of this thesis, aims to achieve precisely this
26
balance.
3.3 Phase Field Crystal Theory
The phase field crystal theory (PFC) presents a solution to the aforementioned numerical dif-
ficulties faced by DDFT methods by approximating the free energy in such a way as to retain
the basic features of the theory using a smoother solid state description of density . Starting
with the approximate free energy functional of equation 2.44 we proceed as previously by
scaling out a factor of the reference density and changing variables to a dimensionless density
n(r) = (ρ(r)− ρl)/ρl,
βF [n(r)]ρl
=
∫dr {(n(r) + 1) ln(n(r) + 1)− (1− βµ0)n(r)} −
1
2n(r) ∗ ρlC(2)0 (r, r′) ∗ n(r′).
(3.23)
We then Taylor expand the logarithm about the reference density or equivalently n(r) = 0,
to fourth order,
βF [n(r)]ρl
=
∫dr
{n(r)2
2− n(r)
3
6+n(r)4
12
}− 1
2n(r) ∗ ρlC(2)0 (r, r′) ∗ n(r′). (3.24)
Where the linear term can be dropped by redefining the density n(r) about its average. Most
phase field crystal theories also use a simplified equation of motion as well,
∂n(r, t)
∂t= M∇2
(δF [n(r)]δn(r)
). (3.25)
As alluded to above, these two simplifications formally make the PFC theory different
from CDFT, turning it instead into a type of Ginzburg-Landau type of field theory, where
n represents an order parameter that becomes periodic in the solid state. As has been
shown in the PFC literature, this apparently gross over-simplification of CDFT manages
to correctly reproduce many of the qualitative physics of solidification, such as nucleation,
27
grain boundary misorientation energy, elastic response and dislocations in the solid phase,
vacancy diffusion and creep, grain boundary pre-melting, vacancy trapping, and numerous
other effects. By progressively improving the parametrization of PFC theories, guided by
inspection of the underlying forms, PFC will be able to better quantitatively model the
aforementioned processes.
28
Chapter 4
Simplified Binary Phase Field Crystal
Models
In this chapter we will review two current simplified binary PFC models. The first is the
original binary PFC model of Elder et al. [3] and the second is the binary structural PFC
(XPFC) model of Greenwood et al. [14]. We begin by establishing background shared by all
binary PFC models and move on to summarize and review each.
4.1 Binary PFC Background
We begin with a multicomponent variant of the approximate free energy functional estab-
lished in Chapter 2,
βF [ρA, ρB] =∑i=A,B
∫dr ρi(r) ln
(ρi(r)
ρ0i
)− (1− βµ0i )∆ρi(r) (4.1)
− 12
∑i,j=A,B
∆ρi(r) ∗ C(2)ij (r, r′) ∗∆ρj(r′).
29
It is convenient to change variables to a dimensionless total density, n(r) and local concen-
tration, c(r),
n(r) =∆ρ
ρ0=
∆ρA + ∆ρBρ0A + ρ
0B
(4.2)
c(r) =ρBρ
=ρB
ρA + ρB. (4.3)
Scaling out a factor of the total reference density, ρ0 we can break the free energy functional
in these new variables into three parts,
βF [n, c]ρ0
=βFid[n]ρ0
+βFmix[n, c]
ρ0+βFex[n, c]
ρ0, (4.4)
where, Fid, Fmix and Fex are the ideal, mixing and excess free energies respectively. These
are defined as,
βFid[n]ρ0
=
∫dr{
(n(r) + 1) ln(n(r) + 1)− (1− βµ0)n(r)}
(4.5)
βFmix[n, c]ρ0
=
∫dr
{(n(r) + 1)
(c ln
(c
c0
)+ (1− c) ln
(1− c1− c0
))}, (4.6)
where we have introduced µ0 = µ0A +µ0B as the total chemical potential of the reference mix-
ture, and c0 = ρ0B/ρ0 as the reference concentration. Assuming that the local concentration
c(r) varies over much longer length scales than the local density n(r), the excess free energy
term becomes
βFex[n, c]ρ0
=− 12n(r) ∗ [Cnn(r, r′) ∗ n(r′) + Cnc(r, r′) ∗∆c(r′)] (4.7)
− 12
∆c(r) ∗ [Ccn(r, r′) ∗ n(r′) + Ccc(r, r′) ∗∆c(r′)] ,
30
where we have introduced and ∆c(r) = c(r)− c0 as the deviation of the concentration from
the reference. The n− c pair correlations introduced in the excess free energy are,
Cnn = ρ0(c2CBB + (1− c)2CAA + 2c(1− c)CAB
)(4.8)
Cnc = ρ0 (cCBB − (1− c)CAA + (1− 2c)CAB) (4.9)
Ccn = Cnc (4.10)
Ccc = ρ0 (CBB + CAA − 2CAB) (4.11)
Explicit derivations of these terms can be found in Appendix C. Differences in the various
simplified binary PFC theories stem from differing approximations of the terms in the free
energy stated in equations 4.5, 4.6 and 4.7.
4.2 Original Binary Phase Field Crystal Model
In the original simplified binary PFC theory, all terms in the free energy are expanded about
n(r) = 0 and c(r) = c0 (ie., about their reference states). For the ideal free energy this
results in a polynomial truncated to fourth order,
βFid[n]ρ0
=
∫dr
{n(r)2
2− ηn(r)
3
6+ χ
n(r)4
12
}. (4.12)
The linear term in the expansion is dropped by redefining n about its average and we
have added the fitting parameters η and χ to fit the free energy away from the reference
parameters. If we assume for simplicity of demonstration c0 = 1/2, the free energy of mixing
becomes a simple fourth order polynomial as well,
βFmix[n, c]ρ0
=
∫dr
{2∆c(r)2 +
4∆c(r)4
3
}. (4.13)
31
Linear couplings to n(r) are dropped by assuming, as we already have, that the concentration
field varies on a much longer length scale than the total density and noting that the total
density is defined about its average. This argument can also be applied to the linear couplings
to n(r) in the excess free energy term, which then leaves only the Cnn and Ccc terms. Finally,
these two terms are approximated with a gradient expansion of the form,
Cnn(r, r′) =
(C0 + C2∇2 + C4∇4 + . . .
)δ(r − r′), (4.14)
Ccc(r, r′) =
(�+Wc∇2 + . . .
)δ(r − r′). (4.15)
The expansion parameters, C0, C2, and C4 are all dependent on temperature and concen-
tration. We are required to expand Cnn to fourth order because, as noted in chapter 3, the
peak of the direct correlation function in Fourier space is the driving force for solidifica-
tion. The concentration field is correlated over a longer length scale implying that only the
short wavevectors are important in Ccc so we can expand just to quadratic order, effectively
treating c as in the traditional Cahn-Hilliard theory.
Gathering terms, the resulting free energy functional for the original simplified binary
PFC model1 is,
βF [n, c]ρ0
=
∫dr
{1
2n(r)
(1− C0 − C2∇2 − C4∇4
)n(r)− ηn(r)
3
6+ χ
n(r)4
12
}(4.16)
+
∫dr
{1
2∆c(r)
(4− �−Wc∇2
)∆c(r) +
4∆c(r)4
3
}.
The strength of the original simplified binary PFC model is that is retains most of the
important physics of binary alloys in a very reduced theory. For instance, the simplified
model is capable of describing the equilibrium phase diagrams of both eutectic alloys and
materials with a solid state spinodal / liquid minimum. Supplied with a diffusive equation
of motion, the simplified model can model an impressive diversity of dynamic phenomena
1The orignal simplified binary PFC model was expressed using slightly different variables. We expand in∆c(r) here to facilitate comparison with other theories
32
including eutectic growth [3], solute segregation [33], dendritic growth [3], epitaxial growth
[11, 12] and crack formation [34].
The major limitation of the original simplified model is that the gradient expansion of the
density-density correlation function gives only a crude control over the crystal structures that
can be formed. In fact, as this theory only controls a single peak in Fourier space it can only
solidify into the BCC phase. As noted in chapter 3, the ability to solidify into an arbitrary
structure demands control of the density-density correlation function at all reciprocal lattice
vectors.
A second limitation of the original simplified model is that it is local in concentration.
This means that realistic phase diagrams from 0 to 100% concentration cannot be produced,
only local phase diagrams around the reference concentration2. The limited concentration
range is problematic for comparing to experimental phase diagrams. To obtain relatable and
testable results, a major motivation for binary XPFC and this work, we require the entire
free energy of mixing term in eqution 4.6.
4.3 Original Binary Structural Phase Field Crystal Model
The binary structural phase field crystal theory (XPFC) seeks to remedy the two short
comings of the original simplified model. That is, it seeks to reproduce a variety of crystal
lattice structure and to construct phase diagrams of a range of concentrations. We’ll begin
with a derivation of the theory and compare with the original model.
First, the ideal free energy is expanded in precisely the same manner resulting in the
same fourth order polynomial,
β∆Fid[n]ρ0
=
∫dr
{n(r)2
2− ηn(r)
3
6+ χ
n(r)4
12
}. (4.12 revisited)
The free energy of mixing is left unexpanded but an overall scale ω is added to fit the mixing
2Indeed, the original model ”concentration” was in fact a density difference, not true concentration.
33
term away from the reference concentration,
βFmix[n, c]ρ0
=
∫dr
{ω(n(r) + 1)
(c ln
(c
c0
)+ (1− c) ln
(1− c1− c0
))}. (4.17)
This unexpanded free energy of mixing will lead to more accurate global phase diagrams.
The excess free energy is approximated using similar assumptions as in the original model
(linear couplings are dropped), but the density-density correlation function, Cnn, is not
expanded. Instead, Greenwood et al all assumed that the k = 0 mode of the concentration-
concentration correlation function was zero leaving only the quadratic term in the expansion,
Ccc(r, r′) = δ(r − r′)Wc∇2. (4.18)
Grouping terms together, the complete free energy functional for the binary XPFC model
is,
β∆F [n, c]ρ0
=
∫dr
{1
2n(r) (1− Cnn(r, r′)) ∗ n(r′)− η
n3
6+ χ
n4
12
}(4.19)
+
∫dr
{Wc2|∇c(r)|2 + ωfmix(r)
}.
Where fmix(r) is the local free energy density of mixing,
fmix(r) = (n(r) + 1)
(c(r) ln
(c(r)
c0
)+ (1− c(r)) ln
(1− c(r)1− c0
)). (4.20)
The density-density correlation function, Cnn, is left unexpanded in Fourier space but
assumed to have a specific phenomenological form,
Cnn = ζA(c)CAA(r, r′) + ζB(c)CBB(r, r
′), (4.21)
34
where ζA(c) and ζB(c) are interpolation functions, assigned the forms
ζA(c) = 1− 3c2 + 2c3 (4.22)
ζB(c) = ζA(1− c). (4.23)
by Greenwood et al.
The remaining elemental correlation functions CAA and CBB are modelled using the
general XPFC model for correlation functions, which we describe subsequently.
4.3.1 XPFC Correlation Functions
The key insight made by the XPFC model is that the density-density correlation function
can be modelled in such a way as to control the crystal lattice structure formed under so-
lidification and to target different structures at different concentrations, and temperatures.
Originally delineated for pure systems, the XPFC method for constructing correlation func-
tions is strongly influenced by the methods developed by Ramakrishnan. In particular this
means that we need a model correlation function that controls the values specifically at the
reciprocal lattice vector positions. We can achieve this with Gaussian peaks centred at the
reciprocal lattice vector positions,
C̃(k) =∑α
eTT0 e− (k−kα)
2
2σ2α (4.24)
Where, as in chapter 3, the index α runs over families of point group symmetry-equivalent
reciprocal lattice vectors, kα is the length of the reciprocal lattice vectors in α and σα
is the width of the peak. Temperature dependence of the correlation peaks is achieved
through the prefactors eT/T0 which gives the correct temperature scaling of the amplitudes
at temperatures much higher than the Debye temperature3 as discussed by [13].
3The original XPFC works used a phenomenological prefactor eσ2/Ci , where σ was considered a model
temperature parameter and Ci a constant. That choice was inspired by harmonic analysis in the solid phase
35
The primary advantages of the XPFC model are two fold: they produce realistic phase
diagrams and they model a variety of crystalline lattices. While the former is relatively
cosmetic the latter allows for the examination of genuinely novel systems in comparison
with the original simplified model. For example, the binary XPFC model has been used to
study peritectic systems [14], ordered crystals [13], dislocation-assisted solute clustering and
precipitation [7, 8] and solute drag [6]. It is noteworthy, that the above works on clustering
have been validated experimentally in binary and ternary alloys.
Figure 4.1: Eutectic phase diagram with metastable projections. Stable coexistance linesare rendered solid whereas metastable projections are dashed.
Unfortunately, by assuming that the k = 0 mode of the concentration-concentration
correlation function is zero, the XPFC model restricts its free energy of mixing to an ideal
model of mixing. This model of mixing includes only entropic contributions to the free
energy. In the solid state, this means that the sole driving force for phase separation is
elastic energy as the enthapy of mixing is always zero. This inhibits the modelling of a
variety of binary alloy systems, for instance both monotectic and syntectic systems cannot
and the Debye-Waller factor.
36
be modelled without a negative enthalpy of mixing. More subtly, in the present XPFC alloy
model, even eutectic systems have a negative heat of mixing deep below the eutectic point
as the metastable liquid has a spinodal. This phenomenon is shown schematically in figure
4.1, where the metastable projections, including solid and liquid spinodals, are drawn on a
hypothetical eutectic phase diagram.
A second disadvantage of the present XPFC model is that the phenomenological form for
the correlation function as seen in equation 4.21 implicitly assumes that there are well defined
structures at c = 0 and c = 1. This works well for modelling eutectic systems for example,
but does not work very well when we expect a solid phase at intermediate concentration.
These shortcomings are the motivation for the improvements developed in this thesis which
are presented in the following chapter.
37
Chapter 5
Improvements to the Binary XPFC
Model
In this chapter we look at two improvements to the binary XPFC theory. Both of these
improvements are novel contributions to the field and significantly extend the scope of the
XPFC framework. The improvements, as previously alluded to, are to first, extend the free
energy of mixing in the XPFC model to one with an enthalpy of mixing and to second,
generalize the phenomenological for of the two-point correlation function in binary alloys.
5.1 Adding an Enthalpy of Mixing
Extending the free energy of mixing beyond ideal mixing is achieved by removing the assump-
tion made by Greenwood et al. in deriving the binary XPFC model that the concentration-
concentration correlation function has no k = 0 mode. This is the same approach taken in
the original PFC model, though here we keep the ideal mixing term unexpanded as in the
original XPFC alloy model. Specifically, the correlation function is expanded as,
Ccc(r, r′) = δ(r − r′)
(ω�+Wc∇2 + · · ·
), (5.1)
38
where � is a parameter that is possibly temperature dependent. This form results in a free
energy functional of the form,
β∆F [n, c]ρ0
=
∫dr
{1
2n(r) (1− Cnn(r, r′)) ∗ n(r′)− η
n3
6+ χ
n4
12
}(5.2)
+
∫dr
{Wc2|∇c(r)|2 + ωfmix(r)
},
where the local free energy density of mixing, fmix is now,
fmix(r) = (n(r) + 1)
(c(r) ln
(c(r)
c0
)+ (1− c(r)) ln
(1− c(r)1− c0
))+
1
2�(c− c0)2. (5.3)
For simplicity the temperature dependence of the parameter � is taken to be linear about a
spinodal temperature Tc,
�(T ) = −4 + �0(T − Tc). (5.4)
The resulting model has a free energy of mixing that is equivalent to the regular solution
model and, as such, it makes a clear connection to a well used model elsewhere in material
science. The regular solution model also supplies the essential physics of a non-negligible
enthalpy of mixing.
5.2 Generalizing the Two-Point Correlation Function
To establish a general phenomenology for modelling density-density correlation functions in
alloys, note that the density-density correlation function has the form of a linear combination
of interpolating functions in concentration, ζ(c), multiplied by bare correlation functions
C(r, r′) of individual components,
Cnn(r, r′; c) =
∑i
ζi(c)Ci(r, r′) (5.5)
39
where the index i is, for the moment, an arbitrary label. For example, in the exact theory that
emerges from the original alloy CDFT theory (equation 4.8), we use the labels {AA,AB,BB}
and have interpolation functions,
ζAA(c) = ρ0(1− c2), (5.6)
ζAB(c) = ρ0c(1− c), (5.7)
ζBB(c) = ρ0c2. (5.8)
This suggests the following new definition that we introduce herein to generalize the density-
density correlation function for a binary alloy: Use the labels i to enumerate the set of crystal
structures known to manifest themselves in an alloy system. The correlation functions,
Ci(r, r′) are then direct correlation functions that model the crystal structure i and the
associated interpolation functions ζi(c) define the range of concentrations over which these
correlations are valid. In principle, ζi(c) can also be temperature dependent, although we do
not consider that case in this thesis.
As a simple example, if we wanted to construct a model of the silver-copper eutectic
alloy system, we might start with some model correlation function for pure silver, Cα(r, r′),
and for pure copper, Cβ(r, r′). These two structures, the silver rich α phase and the copper
rich β phase, are the only two relevant crystalline phases in the system, so to build the full
density-density correlation function we just need to choose interpolating functions for each
phase. Following Greenwood et al. for example, we might choose,
ζα(c) = 1− 3c2 + 2c3, (5.9)
ζβ(c) = 1− 3(1− c)2 + 2(1− c)3. (5.10)
To model the α and β correlation functions we use the original XPFC formalism for modelling
bare correlation functions (i.e. equation 4.24). The α and β phases are both FCC [35] so we
40
can use an FCC model for the correlation function as in [36].
5.3 Equilibrium Properties of Binary Alloys
These two changes to the XPFC formalism extend the possible systems we can study. In this
section we’ll explore the equilibrium properties of the improved XPFC free energy functional
specialized for three different material phase diagrams: eutectic, syntectic and monotectic.
5.3.1 Eutectic Phase Diagram
While previous PFC models have shown that elastic energy is a sufficient driving force for
eutectic solidification, our simplified regular solution XPFC model allows for the examination
of the role enthalpy of mixing can play in eutectic solids. For instance, Murdoch and Schuh
noted that in nanocrystalline binary alloys, while a positive enthaply of segregation can
stabilize against grain growth via solute segregation at the grain boundary, if the enthaply
of mixing becomes too large this effect can be negated by second phase formation or even
macroscopic phase separation[37].
To specialize our simplified regular model to the case of the binary eutectic, we must
choose an appropriate model for the correlation function. Choosing an α phase around c = 0
and β phase around c = 1, we can recover the pair correlation function used in the binary
XPFC of Greenwood et al. with a particular choice of interpolation functions:
ζα(c) = 2c3 − 3c2 + 1 (5.11)
ζβ(c) = ζα(1− c). (5.12)
Should we choose, for example, an α and β phase with 2 dimensional hexagonal lattices,
differing only by lattice constants, we can produce a phase diagram like that in Fig. 5.1.
The phase diagram also depicts the phase diagram of the metastable liquid below the eutectic
41
point showing the binodal and spinodal lines where the metastable liquid becomes unstable
with respect to phase separation. The spinodal line indicates an inflexion point in the free
energy of the metastable liquid where the liquid becomes fully unstable with respect to
phase separation whereas the binodal line indicates the coexistance curve of the decomposed
metastable liquid.
Figure 5.1: Eutectic phase diagram for triangle α and β solid phases and l denotes theliquid. The free energy parameters are η = 2, χ = 1, ω = 0.02, �0 = 26.6 and Tc = 0.15.The parameters of the structure functions are σ10α = σ10β = 0.8, k10α = 2π, k10β = 4π/
√3
and T0 = 1. The horizontal line denotes the eutectic temperature.
It is noted that the phase diagram in Fig. 5.1 and in what follows were done using the
same approach that was used in numerous PFC literature [14]. The approach is as follows:
a mode expansion for the density is assumed for each crystal phase (zero amplitudes for
the liquid phase). For each phase, an amplitude equation analogous to equation 3.6 results,
except in this case, it is a function of amplitudes, average density and concentration. This
coarse grained free energy of each phase is then minimized with respect to the amplitudes,
42
leaving a free energy density for each phase that is a function only of the average density
and concentration. At this juncture, we simplify matters by assuming that the average
density is a constant for the system. We then minimize the total free energy of the system
with respect to concentration, assuming a conserved total concentration field. This latter
step considers separately the coexistence of (1) α-liquid, (2) β-liquid, (3) α-β over different
temperature/concentration ranges. Original code was developed to carry our these phase
diagram constructions, and implemented using Julia [38], Maxima.jl [39] and the Maxima
symbolic computation engine [40].
5.3.2 Syntectic Phase Diagram
Our improved XPFC model also allows for the study of a variety of invariant binary reactions
that, to date, have not been studied using phase field crystal models. One such reaction is
the syntectic reaction.
The syntectic reaction, l1+l2 → α, consists of solidification at the interface of two liquids.
We can achieve this with our model by setting the spinodal temperature, Tc, in equation
5.4 sufficiently high and producing a density-density correlation function that is peaked at
a concentration below the spinodal. This can be done by choosing a single interpolation
function to be a window function that is centered about an intermediate concentration, cα
of the solid phase, α. One obvious choice is,
ζ(c) = e− (c−cα)
2
2α2c (5.13)
The resulting correlation function for a hexagonal lattice in a syntectic alloy in two dimen-
sions becomes,
C̃nn(k; c) = e− (c−cα)
2
2α2c e− TT0 e−
(k−k′)2
2α2 (5.14)
A phase diagram that produces a syntectic reaction with an appropriate choice of parameters
can be seen in Fig. 5.2.
43
Figure 5.2: Phase Diagram of Syntectic Alloy with a hexagonal solid phase α. The freeenergy parameters are η = 2, χ = 1, ω = 0.3, �0 = 10 and Tc = 0.35. The parameters forthe structure function are α10α = 0.8, k10α = 2π and T0 = 1. The horizontal line denotes thesyntectic temperature.
5.3.3 Monotectic Phase Diagram
The monotectic reaction is another invariant binary reaction that has not previously been
studied using PFC models. The monotectic reaction, l1 → α + l2, consists of decomposing
liquid into a solute poor solid and solute rich liquid. To model a monotectic using our im-
proved XPFC model we hypothesize a solid phase at c = 0 and set the spinodal temperature
higher than the solidification temperature. To achieve this, we use a window function peaked
around c = 0,
χα(c) = e− c
2
2α2c . (5.15)
Again considering a simple hexagonal lattice for the α phase, we can produce a phase diagram
with a monotectic reaction with an appropriate choice of parameters as in Fig. 5.3.
44
Figure 5.3: Phase Diagram of Monotectic Alloy with hexagonal α phase. The free energyparameters are η = 2, χ = 1, ω = 0.3, �0 = 10, Tc = 0.35 and c0 = 0.75. The parametersfor the structure function are α10α = 0.8, k10α = 2π and T0 = 1 and the parameter for thewindow function is αc = 0.4. The horizontal line indicates the monotectic temperature.
The improvements to the XPFC formalism made in this chapter not only reveal new
details in existing systems, but also model new systems that haven’t been explored with
PFC methods before. They provide a general framework to explore the landscape of other
possible binary alloys with an emphasis that the liquid free energy is a crucial element in this
complete description. It is also noteworthy that the approach introduced here is extendable
in a straightforward way to multi-component alloys if the interpolation functions become
multivariate functions of the concentrations.
45
Chapter 6
Applications
In this chapter we discuss applications of the improved binary XPFC model introduced in
Chapter 5 to an application in microstructure evolution. To begin, we introduce a phe-
nomenological set of equations of motion that describe solute and density diffusion in the
binary XPFC model. We then apply these to the examination of the process of diffusion lim-
ited precipitation from solution. Recent experimental work on the precipitation of gold and
silver nanoparticles [1] and on the precipitation of calcium carbonate [2] has demonstrated
that the pathway to nucleation can deviate highly from the approximations of Classical Nu-
cleation Theory (CNT). Specifically, both experiments observe spinodal decomposition of the
solution prior to nucleation in the solute rich phase. In this chapter, we’ll present early find-
ings from our new model that lend support for this dynamical behaviour and, additionally,
show that the growth behaviour post-nucleation may be more complex than usual diffusive
growth and coarsening typically observed. To conclude we discuss future applications both
in the study of precipitation and other areas.
46
6.0.1 XPFC Dynamics
To examine applications of our improvements to the XPFC model we begin by considering
equations of motion. Following [14], we use conservative dynamics for both n(x, t) and c(x, t).
∂n(x, t)
∂t= Mn∇2
(δβ∆F/ρ0δn(x, t)
)+ ξn(x, t), (6.1)
∂c(x, t)
∂t= Mc∇2
(δβ∆F/ρ0δc(x, t)
)+ ξc(x, t), (6.2)
where Mn and Mc are the solute and density mobilities. The noise terms ξn(x, t) and ξc(x, t)
model thermal fluctuations. Their dynamics follow the fluctuation-dissipation theorem, the
theory of which is derived in the Appendix A. These equations of motion are largely phe-
nomenological as, strictly speaking, there is no reason that the local concentration should
be conserved. This conservation can be justified in the limit that the total density does not
deviate far from the reference. When this is the case we have c ≡ ρB/ρ ≈ ρB/ρ0 which is
conserved. For simplicity, we will carry out simulations in this chapter in this limit.
6.1 Multi-Step Nucleation of Nanoparticles in Solution
Many nanoparticle solutions are formed by precipitation from solution and their size distri-
bution (polydispersity index) is of key importance to their application. Therefore, a precise
understanding of the kinetic pathway of precipitation is of crucial importance in designing
synthesis techniques of highly mono-disperse nanoparticles.
As stated above, recent experimental work has shown that precipitation from a solu-
tion can follow a pathway vary different from that assumed by Classical Nucleation Theory
(CNT) [1, 2]. CNT assumes that, for binary systems, changes in composition occur simul-
taneously with changes in order. In contrast, these experimental findings suggest that in
certain systems changes in composition can precede changes in order via spinodal decompo-
sition. While there is some dispute about whether or not to call this process a non-classical
47
nucleation pathway [41, 42], the observed pathway to precipitation raises several questions
about its classification, regardless of semantics.
6.1.1 Classical and Non-classical Nucleation Theories
In CNT, the rate of formation of post-critical can be written as an Arrhenius equation,
J =∂n∗
∂t= Ae−β∆G
‡, (6.3)
where,
A is a constant prefactor,
∆G‡ is the Gibbs free energy of a critical nucleus and,
n∗ is the number of critical nuclei.
Following [43], the probability of nucleation of a droplet of volume V , fnuc(t), is then,
fnuc(t) =
〈NcryNtotal
〉= 1− e−JV t, (6.4)
where Ncry and Ntotal are the number of crystalline droplets and the total number of droplets
respectively.
CNT assumes that there is a single critical state which is specified by the thermody-
namic parameters of the target phase at a critical radius R∗. This naive approach dramat-
ically underestimates the time required to assemble a critical nucleus due to its simplistic
parametrization of the kinetic pathway [43–45].
Improvements to CNT can be made to the model by increasing the parameter space
describing the nucleation process. Considering both radius and density of the critical nucleus
[44] gives good agreement with nucleation of globular proteins, for example. One problem
with this approach is the selection of appropriate parameters. There is no guarantee that
48
a finite set parameters will describe the kinetic pathway taken by a nucleus and if we are
without a fundamental technique for calculating the chosen parameters we have little way
of knowing if our theory is accurate or simply over-fit. In [45], for example, nucleation data
is fit to the functional form instead of using calculated or otherwise measured parameters.
Statistical field theories such as the XPFC alloy model can help provide an answer to
this problem by taking an unbiased approach to nucleation process within the context of
CDFT. The critical state, and entire kinetic pathway, can be examined free of any particular
parametrization. The equations of motion can be integrated numerically for an ensemble
systems and nucleation details measured from the computed results. Moreover, unlike other
numerical approaches to nucleation like molecular dynamics or formal density functional
theory, the PFC model can examine nucleation on diffusive time scales.
6.1.2 XPFC Modelling of Precipitation
To construct an appropriate free energy functional for a system analogous to gold nanopar-
ticles studied by Loh et al. [1] we consider the structure of its equilibrium phase diagram.
Precipitation is indicative of a simple liquid-solid coexistance curve. The presumed pres-
ence of spinodal decomposition under certain circumstances indicates that it is a metastable
liquid spinodal submerged beneath the liquid-solid coexistance curve [41]. We assume that
there must exist conditions under which the spinodal decomposition of the metastable liquid
phase occurs more rapidly than nucleation directly from solution (ie., classical nucleation).
Producing a phase diagram in our XPFC model with these characteristics is very similar
to modelling a monotectic system with the exception that the spinodal temperature Tc must
be low enough to hide the entire liquid spinodal below the coexistance curve. We will also
centre the interpolation function ζα(c) about c = 1 so that the nanocrystalline solid α is
favoured at large concentration. The resulting density-density correlation function for a 2
49
dimensional hexagonal precipitate would thus be,
C̃nn(k; c) = exp
{−(c− 1)
2